### 3D between vibrational dynamics and structural relaxation

C A Massa1, D Leporini1,2and F Puosi2

1_{Istituto per i Processi Chimico-Fisici-Consiglio Nazionale delle Ricerche (IPCF-CNR), via}
G. Moruzzi 1, 56124 Pisa, Italy

2_{Dipartimento di Fisica “Enrico Fermi”, Universit`a di Pisa, Largo B. Pontecorvo 3, 56127}
Pisa, Italy

E-mail: [email protected]

Abstract.

Glass-forming systems approaching their glass transition exhibit universal correlations between picosecond vibrational dynamics and long-time structural relaxation, which can be described by the same master curve in the bulk or confined conditions. In this work, we study at a fundamental level the effects of the reduction of spatial dimensionality on this phenomenon. We perform Molecular Dynamics simulations of a metallic glass-formers in two dimensions (2D). We show that in the supercooled regime particle localization in the cage and structural relaxation are blurred by long-wavelength fluctuations specific to low-dimensional systems. Once these effects are properly removed, we demonstrate that the fast dynamics and slow relaxation comply, without any adjustment, with same scaling between the structural relaxation time and the Debye-Waller factor, originally observed in three-dimensions (3D).

In glass-forming liquids approaching the glass transition (GT), the huge slowing-down of structural relaxation and the increase of viscosity is accompanied by the localization of their constituent atoms and molecules, which are increasingly trapped by their surroundings, a phenomenon usually indicated as cage effect. Localization is quantified by the Debye-Waller (DW) factor hu2i, i.e., the mean square amplitude of particle motion on a picosecond timescale. In the last decade numerous evidences have been reported supporting the existence of a link between the long-time structural relaxation time ταand the fast dynamics as denoted

by hu2i. Correlations have been found in simulations of model systems such as polymers
[1, 2, 3], binary mixture [4], water [5, 6] and metallic liquids [7, 8] and validated with
experimental data on several glass-formers [1, 9, 10, 3]. Further, it was also shown that
the fast dynamic property hu2_{i encodes some basic aspects of the dynamic slowing-down as}

approaching the GT like the onset of mechanical rigidity[11], the development of dynamical heterogeneities (DHs) and the break-down of the Stokes-Einstein relation [12,8] .

Remarkably, the correlation between fast dynamics and relaxations is not limited to bulk materials, where it was originally evidenced, but extends to non-bulk conditions. In simulations of supported thin films, Douglas and coworkers showed that, by considering the average dynamics of the film, the bulk-like scaling law between hu2i and ταis recovered with

a slightly different scaling adjustable parameter [13]. Taking into account the strong gradient
of mobility in the film via a layer resolved analysis, Leporini and coworkers improved on
previous results and showed that the hu2_{i-τ}

α correlation is exactly the same of bulk, i.e., it

is described by the same master curve with no adjustable parameters [14]. These findings suggest that the dynamics in thin films or confined materials and in their bulk counterpart are controlled by the same fundamental rules. To support this idea, we mention a recent work on a polymeric liquid under 1D and 2D nanoconfinement where the authors shows that the exponent for the density scaling of the segmental relaxation time is not affected by the confinement dimensionality and size and agrees with the value from bulk measurements [15]. Motivated by these results, in the present work we study, via Molecular Dynamics (MD) simulations in two dimensions (2D), the impact of the reduction in spatial dimensionality on the scaling between fast dynamics and relaxation. Here we focus on a model of liquid metal, Cu50Zr50, which is known to have the best glass-forming ability among binary metallic

systems in three dimensions (3D) [16]. In agreement with previous works [17, 18], we find
that both fast dynamics localization and structural relaxation are affected by long-wavelength
fluctuations specific to low-dimensional systems. If these effects are properly treated, the
scaling between hu2_{i and τ}

αis recovered which exhibit the same master curve observed in 3D

bulk with no adjustable parameters.

The paper is organized as follows. In Sec.2details about the numerical models are given. The results are presented and discussed in Sec. 3and the main conclusions are summarized in Sec.4.

2. Methods

MD simulations for the CuZr binary alloy were carried out in 2D using LAMMPS molecular dynamics software [19]. An embedded atom model (EAM) potential was used to describe the interatomic interactions [20]. Each simulation consists of a total number of N = 3200 atoms contained in a box with periodic boundary conditions. The equations of motion are integrated using the velocity Verlet algorithm with a time δt which ranges in 10−4− 2 × 10−3ps. The temperature T is defined from the kinetic energy, T = PN

i mi|vi|
2_{/2N k}

B, where vi and mi

are the velocity and mass of the ith atom and kBis the Boltzmann constant. The pressure P is

defined via the virial, P = ρkBT + 1/2V

D P

i<jfij· rij

E

, where ρ is the number density, V the volume and fijis the force between atoms i and j at distance rij.

Supercooled samples at different temperatures were generated with the following protocol. Initial configurations were equilibrated at 2000 K, rapidly quenched directly at the target temperature and then equilibrated in the NPT ensemble at zero pressure for a time sufficient to remove all the transient effects in energy and dynamics (order of 100τα).

Production runs were carried out in the NVE ensemble,which extend in time until the onset of diffusive regime. With the same protocol, we also carried out simulations under positive external pressure, P = 5 GPa and P = 10 GPa (if not mentioned, in the following discussion data refers to P = 0 conditions). Ten to twenty independent realizations of each state were considered to ensure suitable statistical average.

3. Results and discussion

3.1. Structural characterization of the supercooled state

First, we study the evolution of the liquid structure in the supercooled state as denoted by global radial distribution function g(r) and the static structure factor S(q), defined as:

g(r) = 1 2πr∆rρ(N − 1) * X j6=i δ(|rij| − r) + (1) S(q) = 1 N * X i X j e−iq(rj−ri) + (2)

where ri is the position of the ith atom, rij = rj − ri and h...i denotes the ensemble

average. In Figure 1g(r) and S(q) are shown for selected temperatures. The lack of long-range translational order, typical of the supercooled liquid state, is apparent in both the quantities. On the other hand, the splitting of the second peak developing upon cooling could be the signature of the emergence of medium-range ordering. For the present model, Hu et al. demonstrated that in 2D growing local crystal-like order controls the slowing-down of dynamics in the supercooled liquid and play a crucial role in the formation of a 2D metallic glass. [21].

0 1 2 3 4 5 6 7 8 q [Å-1] 0 1 2 3 4 5 6 7 8 S(q) 0 5 10 15 r [Å] 0 1 2 3 4 5 6 7 g(r) 750 K 775 K 850 K 1000 K 1200 K 1500 K 2000 K

Figure 1. Radial distribution functions g(r) (top panel) and structure factors S(q) (bottom panel) at selected temperatures. The data have been shifted for clarity.

0 0.2 0.4 0.6 0.8 1 j 6 0 0.5 1 1.5 2 2.5 3 3.5 P( j ) 6 750 K 775 K 850 K 1000 K 1200 K 1500 K 2000 K Cu Zr

Figure 2. Distribution P (ψj_{6}) of the hexatic-order parameter ψ6jfor Cu atoms (dash-dotted
lines), Zr atoms (dashed lines) and global (solid lines), at selected temperatures.

In order to deepen the structural aspects, we consider the hexatic-order parameter ψ_{6}j:

ψ_{6}j = 1
nj
nj
X
m=1
ei6θ(rmj)
(3)

where θ(rmj) is the angle between rmj = rm− rj and the x axis, nj is the nearest neighbors

number of jth atom. Figure 2 displays the temperature dependence of the ψ_{6}j distribution
P (ψ_{6}j) for Cu and Zr atoms. At high temperature ψ_{6}j is broadly distributed and P (ψj_{6}) does
not exhibit any peculiar feature. At lower temperature, a peak appears for large ψ_{6}j values,
corresponding to high local bond orientational order (BOO), that becomes more pronounced
at deeper supercooling. The distribution becomes bimodal, with a minimum occurring at
ψ_{6}∗ = 0.645. This signals the presence of structural heterogeneities, in agreement with the
results of Hu and coworkers [21]. This tendency of increasing BOO is also clear in Figure

3 where we compare two snapshots of the spatial distribution of ψ_{6}j at high (top) and low
(bottom) temperature. At low T we observe some spatially extending regions of high BOO
which are not detected at high temperature. This regions should not be confused with crystal
nuclei developing in a crystallizing system as the former are characterized by a finite lifetime
and their contribution does not increase in time, i.e., the corresponding distribution P (ψ_{6}j) in
Figure2is stationary.

Figure 3. Representative spatial distribution of the hexatic-order parameter ψj6 for T = 2000 K (top) and T = 750 K (bottom).

3.2. Slowing-down of dynamics: localization and structural relaxation

In this section we investigate the slowing-down of dynamics in the supercooling regime, focusing on the two aspects, particle localization and structural relaxation. Atomic mobility is evaluated via the mean square displacement (MSD):

h∆r2(t)i = 1
N
* _{N}
X
j=1
krj(t) − rj(0)k2
+
(4)

The structural relaxation is conveniently described by the self part of the intermediate scattering function (ISF):

Fs(q, t) =
1
N
D_{X}N
j=1
eiq·(rj(t)−rj(0))
E
(5)

The structural relaxation time τα is defined via Fs(qmax, τα) = 1/e where qmax is q-vector

of the maximum of the static structure factor corresponding to about the distance of nearest-neighbors.

In Figure4we plot for selected temperature the MSD (panels A and B) and ISF (panels C and D) of Cu and Zr atoms. We note that the MSD and ISF curves manifest the features which are peculiar of glassy dynamics in 2D and mark the difference with the 3D analogue. Particle localization corresponding to the cage effect, apparent in 3D at low temperature, is virtually absent in 2D. Indeed, the intermediate time plateau is not observed in the ISF and is replaced by a sub-diffusive regime in the MSD. Structural relaxation is also different in 2D and 3D: the quasi-exponential decay of the ISF in 3D is replaced by an extremely slow decay in 2D in which the noise level seems amplified even though the average over 20 independent realizations was considered to improve the statistical precision. These observations agree with previous findings in simulations of binary disks interacting via a Lennard-Jones [17] or soft-core potential [22] as well as experiments on quasi-2D colloids [18] and hard-spheres [23].

For sake of completeness, we consider the non-gaussian parameter (NGP)[24]:

α2(t) =

h∆r4_{(t)i}

(1 + 2/d)h∆r2_{(t)i}2 − 1 (6)

where h∆r4_{(t)i is the mean fourth displacement} _{and d the spatial dimension}_{. The NGP}

quantifies the deviations from the gaussian character of the displacement ascribed to dynamic heterogeneities (DHs). The insets of panel A and B in Fig.4display the NGP of Cu and Zr atoms. We note that, despite the low temperature values attained, the peak value of the NGP, α2,max, remains rather low, α2,max < 1, indicating a modest degree of heterogeneity.

It is now well established that long-wavelength fluctuations, known as Mermin-Wagner fluctuations, are responsible for the vanishing of the transient solid-like dynamics in the supercooled regime [25]. To disentangle the influence of these fluctuations on glassy dynamics, it has been proposed to consider cage-relative (CR) particle motion, namely to measure for each atom the displacement relative to the cage of its neighbors. In this spirit, we define a CR particle displacement:

100 < r 2 (t)> [Å 2 ] 100 0 0.5 1 2 (t) 100 0 0.5 1 2 (t) 100 105 t [ps] 0 0.2 0.4 0.6 0.8 1 F s (q max ,t) 750 K 775 K 800 K 850 K 875 K 900 K 950 K 1000 K 1100 K 1200 K 1300 K 1500 K 1700 K 2000 K 100 105 t [ps] 750 K 775 K 800 K 850 K 875 K 900 K 950 K 1000 K 1100 K 1200 K 1300 K 1500 K 1700 K 2000 K A) B) C) D)

Figure 4. Panels A and B: mean square displacement h∆r2(t)i of Cu (A) and Zr (B) atoms at selected temperatures. Insets: corresponding non-gaussian parameters α2(t). Panels C and D: corresponding self part of the intermediate scattering function Fs(q, t) of Cu (C) and Zr (D). The q-vector qmaxcorresponding to the maximum of the static structure factor is considered.

where ∆rC,j(t) = 1 Nj Nj X i=1 (ri(t) − ri(0)) (8)

The sum in Eq. 8runs over all the nearest neighbors of the jth atom, i.e. the atoms whose distance from the central one at time 0 is smaller than the value corresponding to the first minimum in the g(r). Then, we introduce a CR mean square displacement (CR-MSD):

h∆r2
CR(t)i =
1
N
* _{N}
X
j=1
k(rj(t) − rj(0)) − ∆rC,j(t)k2
+
(9)

and a CR intermediate scattering function (CR-ISF):

Fs,CR(q, t) = 1 N DXN j=1 eiq·(rj(t)−rj(0)−∆rC,j(t)) E (10)

A CR non-gaussian parameter (CR-NGP) can also be defined by replacing in Eq. 6h∆r2_{(t)i}

and h∆r4_{(t)i with the corresponding CR quantities h∆r}2

CR(t)i and h∆r

4

100
105
<
r CR
2
(t)> [Å
2 ]
**Cu**
100
0
1
2
CR 2
(t)
**Zr**
100
0
1
2
CR 2
(t)
100 105
t [ps]
0
0.2
0.4
0.6
0.8
1
F s,CR
(q
max
,t)
750 K
775 K
800 K
850 K
875 K
900 K
950 K
1000 K
1100 K
1200 K
1300 K
1500 K
1700 K
2000 K
100 105
t [ps]
750 K
775 K
800 K
850 K
875 K
900 K
950 K
1000 K
1100 K
1200 K
1300 K
1500 K
1700 K
2000 K
A) B)
C) D)

Figure 5. Panels A and B: cage-relative mean square displacement h∆r2

CR(t)i of Cu (A)

and Zr (B) atoms at selected temperatures. Insets: corresponding cage-relative non-gaussian parameters αCR

2 (t). Panels C and D: corresponding cage-relative self part of the intermediate scattering function Fs,CR(q, t) of Cu (C) and Zr (D). The q-vector qmaxcorresponding to the maximum of the static structure factor is considered. Full circles mark the cage lifetime τc (see the text for more details).

In Figure 5 we show the CR-MSD (panels A and B), the CR-ISF (panels C and D) and CR-NGP (insets of panels A and B) of Cu and Zr atoms for selected temperatures (for comparison, the corresponding standard MSD, ISF and NGP curves are shown in Figure 4). As expected, if we assume the CR perspective, the dynamical signature of the supercooled state, in particular localization and structural relaxation, emerge and it is virtually impossible to distinguish the 2D system from its 3D counterpart only by visual inspection(see [16] for the data of the 3D system).

A crucial aspect of the CR approach is how far in time one can push its validity. Indeed, we expect that, after a given time, due to cage breaking and diffusive processes, one atom will necessarily have lost those neighbors which were detected at time 0. To deepen this aspect, we consider for a given atom the fraction φ(t) of its original neighbors which are still present in the cage after a time t. We define a cage lifetime τc as φ(τc) = (¯nNN − 4)/¯nNN where

¯

n_{NN} ≈ 7 is the mean number of nearest neighbors. This criterion set the vanishing of the cage
when at least 4 initial neighbors are lost, building on the observation that this is the minimum

mark the cage lifetime τcon the CR-MSD and CR-ISF curves in Figure5, we observe that it

occurs when the final decay of the CR-ISF, denoting structural relaxation, is completed. Being the purpose of the present work to discuss the connection between fast dynamics within the cage and structural relaxation, in the following we will consider mainly cage relative dynamical properties. Hence, we define the cage relative Debye-Waller (CR-DW) factor hu2

CRi = h∆r

2

CR(tDW)i where tDW is a measure of the trapping time of a particle in the

cage [1,4]. In agreement with the corresponding 3D model, we set tDW = 1 ps as it ensures

that, at sufficiently low temperature, hu2_{CR}i corresponds to the plateau value of the mean square
displacement denoting particle caging. Similarly, the cage relative structural relaxation time
τCR

α is defined via Fs,CR(qmax, ταCR) = 1/e.

Figure 6 shows the temperature dependence of hu2_{CR}i (panel A) and τCR

α (panel B) for

Cu and Zr atoms. We observe that the CR-DW extrapolates to zero at a finite temperature, T0,DW ≈ 510 K for Cu and T0,DW ≈ 470 K for Zr, in agreement with previous results in 3D

metallic systems [27,16] and polymers [28]. Further, in the supercooled regime the behavior of the CR structural relaxation time can be described by the Vogel-Fulcher-Tamman (VFT) equation, τCR

α = τ0exp[BT0/(T − T0)]. The fitted values of T0, T0 ≈ 565 K and T0 ≈ 550 K

for Cu and Zr atoms respectively, with their uncertainty, compares well with the values of
T_{0,}_{DW from the CR-DW factor.}

3.3. Scaling between fast dynamics and relaxation

Extensive simulation works and experiments revealed strong correlations between fast vibrational dynamics and structural relaxation, which can be expressed as a master curve τα = F (hu2i), connecting the Debye-Waller factor hu2i and the structural relaxation time τα.

Here, we consider the master curve proposed by Larini et al. [1]:

τα = τ0exp
a2
2hu2_{i} +
σ_{a}22
8hu2_{i}2
!
(11)

where τ0, a2and σa22 are system-dependent parameters. Eq.11improves the relation originally

proposed by Hall and Wolynes [29] and accounts for the convexity of the master curve, evidenced by experiments and simulations. Eq.11is recast in the universal form:

τα = ˜τ0exph ˜β(u2g/hu

2_{i) + ˜}

γ(u2_{g}/hu2i)2i (12)

being u2_{g} the DW factor at GT (defined via τα = 102s or η = 1012Pa · s) [1]. In particular,

now the universal constants ˆβ = ˜β ln 10 = 3.7(1) and ˆγ = ˜γ ln 10 = 28.4(2) are introduced, with ˜β and ˜γ defined in [1], and τ0 ensures τα = 102s at GT [1]. Indeed, Eq. 12was shown

to provide a good description of experimental data in several systems [1,9,4].

Figure7is a correlation plot between the structural relaxation time and the inverse DW factor, both quantities derived from cage-relative dynamics, for Cu and Zr components. To test the robustness of this correlation, in addition to the simulation data at zero pressure discussed above, in Fig. 7 we also include data obtained imposing an external pressure on

### 800

### 1000

### 1200

### 1400

### 1600

### 1800

### 2000

### T [K]

### 0

### 0.5

### 1

### 1.5

### <u

CR 2### > [Å

2### ]

### Cu

### Zr

### 0.4

### 0.6

### 0.8

### 1

### 1.2

### 1.4

### 1000/T [K

-1### ]

### -0.5

### 0

### 0.5

### 1

### 1.5

### 2

### 2.5

### log(

CR### [ps])

## A)

## B)

Figure 6. Panel A: temperature dependence of CR-DW factor hu2CRi for Cu and Zr atoms.

The full lines correspond to the linear fit in the low temperature range. Panel B: Arrhenius plot of the CR structural relaxation time τCR

α for Cu and Zr atoms. Full lines are fitted with the Vogel-Fulcher-Tammann (VFT) law τCR

### 0

### 1

### 2

### 3

### 4

### 5

### 6

### 7

### 8

### 9

### (<u

_{CR}2

### >)

-1### [Å

-2### ]

### -0.5

### 0

### 0.5

### 1

### 1.5

### 2

### 2.5

### 3

### log(

CR### [ps])

### Cu, 0 GPa

### Cu, 5 GPa

### Cu, 10 GPa

### Zr, 0 GPa

### Zr, 5 GPa

### Zr, 10 GPa

0 2 4 (<u2>)-1 [Å-2] -1 0 1 log( ) [ps]Figure 7. Main panel: correlation plot of the CR structural relaxation time τCR

α and CR-DW

factor hu2_{CR}i of Cu and Zr atoms. Data for different pressure conditions are shown. Dashed
lines are fitted with the master curve defined in Eq. 11. Inset: corresponding correlation plot
of the usual structural relaxation time ταand DW factor hu2i (see the text for more details).

the system. The superimposed curves are the best-fit with Eq.11, restricted to those states for which log τCR

α ≥ 0.5, i.e., structural relaxation is reasonably separated from the fast dynamics

timescale. We note that Eq. 11 satisfactorily account for the correlation between τCR

α and

hu2

CRi.

Douglas and coworkers [3], building on free-volume arguments, developed a localization model predicting an alternative master curve log τα ∝ hu2i−α/2 where the exponent α would

equal the spatial dimensionality for regular volume shapes, like a sphere in 3D or a circle in 2D. Then, according to this picture, the dependence of τα on hu2i is different in 2D and 3D.

Our results seem not to support this scenario, as we have shown that a 2D system obeys the same scaling law which was derived for 3D systems.

The inset of Fig. 7 presents an alternative analysis of the correlation, in which the
usual DW factor hu2_{i and structural relaxation time τ}

α are examined. The standard scaling

is significantly different from the CR one, being all the data compressed in the short τα and

large hu2i region. Anyway, this approach is at least questionable since, as we discussed above, these quantities are not good estimates of particle localization or structural relaxation.

### 0

### 0.05

### 0.1

### 0.15

### 0.2

### 0.25

### 0.3

### 0.35

### 0.4

### (<u

CR,g 2_{>/<u}

CR
2 _{>)}

### -0.5

### 0

### 0.5

### 1

### 1.5

### 2

### 2.5

### 3

### 3.5

### log(

CR### [ps])

### Cu-2D

### Zr-2D

### Cu-3D

### Zr-3D

Figure 8. Universal scaling between the structural relaxation time and the DW factor. Data for the 2D and 3D models of the metallic glass-forming liquid are shown. The dashed line is the universal master curve, defined in Eq.12.

In Figure8we plot the CR structural relaxation time as a function of the rescaled variable hu2

CR,gi/hu2CRi where hu

2

CR,gi is the value of the CR-DW factor at the glass transition. Following

previous approach [1], we estimate the value of hu2

CR,gi by extrapolating Eq. 11; this yields

hu2

CR,gi = 0.049 ˚A 2

for Cu and hu2_{CR}_{,g}i = 0.045 ˚A2for Zr. We complement the results from the
2D model of metallic liquid with the data for equivalent 3D model, taken from [8]. Simulation
data are compared with Eq.12with no adjustment.

Figure 8 is the major result of the present work. The collapse of the data evidences that structural relaxation and vibrational dynamics of the 2D metallic liquid exhibit the same scaling of 3D systems. The scaling form given by Eq. 12, originally found in bulk and confined 3D systems, also works as a master curve in 2D.

3.4. Density scaling

Finally, we discuss the correlation between fast dynamics and relaxation within the framework of the so-called density scaling. In the past decades, following the advent of high-pressure experiments, a remarkable result in understanding the relaxation and the transport of

### glass-0

### 0.5

### 1

### <u

CR 2### > [Å

2### ]

Cu### = 3.60

Zr### = 3.26

### 0

### 0.5

### 1

### 1.5

### 2

### 2.5

### TS [K Å

2### ]

### 10

6### -0.5

### 0

### 0.5

### 1

### 1.5

### 2

### 2.5

### log(

CR### [ps])

Cu, 0 GPa Cu, 5 GPa Cu, 10 GPa Zr, 0 GPa Zr, 5 GPa Zr, 10 GPa### A)

### B)

Figure 9. Density scaling of the CR-DW factor hu2CRi (panel A) and CR structural relaxation

time τCR

α (panel B). The values of the scaling exponents are γCu= 3.60 and γZr= 3.26.

forming liquids was the discovery that evolution of the structural relaxation time or the viscosity, measured under different T and P conditions, can be described through a simple scaling relation, T ρ−γ or equivalently T vγ, where ρ and v are the density and specific volume (see [30] for a review on this topic). Both the exponent γ and the specific master curve are system-dependent. Even though the density scaling has been mostly investigated on the time scale of the structural relaxation or viscous flow, it was also observed on shorter time scales,

in particular those pertaining to fast dynamics. Density scaling of the DW factor has been reported by previous MD studies in molten salt CKN [31], polymers [28, 32] and binary atomic mixtures [4].

On this basis, we are interested in testing the density scaling in the present model of 2D metallic glass-forming liquid. This is done in Figure9, where we demonstrate the validity of the scaling by plotting the CR-DW factor hu2

CRi (top panel) and the CR structural relaxation

time τCR

α (bottom panel) as a function of the product T Sγ (in 2D the volume is replaced by

the area S). We fix the exponent γ focusing on the fast dynamics: we assume a polynomial
dependence of hu2_{CR}i on T Sγ _{and we determine the value of γ for which the coefficient of}

determination R2of the fit is maximum. Figure9indicates that the density scaling of the fast dynamics leads to the scaling of the structural relaxation with the same exponent, suggesting that also in 2D systems the density scaling is rooted in the fast dynamics, in agreement with previous results in 3D [28].

4. Conclusions

We studied by MD simulations in two dimensions a model of metallic glass-former, CuZr, which is known to possess the best glass-forming ability in three dimensions. In the supercooled regime, while local crystal-like order develops, long wavelength fluctuations wash out caging effects and glassy structural relaxation, which however are recovered if atomic cage-relative dynamics is considered. We have demonstrated that (i) the structural relaxation time exhibits strong correlation with the fast vibrational dynamics, as accounted for by the DW factor of the atoms, and (ii) the correlation is the same of 3D systems, in the sense that it is described by the same master curve, with no adjustable parameters, originally proposed for 3D bulk materials.

Our results in 2D confirm the robustness of the scaling between fast dynamics and slow relaxation. In particular, they provide the basis for understanding the observations of a bulk-equivalent scaling in confined systems [14], as the dynamics within a layer can be considered quasi-2D. Further, Hu et al. in a recent paper showed that for the present model there can be a significant influence of spatial dimensionality on the structural mechanism of glass transition in metallic glasses [21]. Our findings suggest that, despite these structural differences can play a relevant role on both vibrational dynamics and relaxation, they do not affect the deeper aspects of their correlation.

Finally, we note that there is not direct and trivial relation between the present analysis and previous works addressing the effect of spatial dimension in the dynamics of glassforming liquids [13, 14, 15]. Hence, the reported equivalence of 2D and 3D scaling is a further indication supporting the idea that the dynamics in bulk and confined glassforming liquids can be described by the same fundamental rules.

[1] L. Larini, A. Ottochian, C. De Michele, and D. Leporini. Universal scaling between structural relaxation and vibrational dynamics in glass-forming liquids and polymers. Nature Physics, 4:42–45, 2008. [2] F. Puosi and D. Leporini. Scaling between relaxation, transport, and caged dynamics in polymers: From

cage restructuring to diffusion. J.Phys. Chem. B, 115:14046–14051, 2011.

[3] D. S. Simmons, M. T. Cicerone, Q. Zhong, M. Tyagi, and J. F. Douglas. Generalized localization model of relaxation in glass-forming liquids. Soft Matter, 8:11455–11461, 2012.

[4] F. Puosi, C. De Michele, and D. Leporini. Scaling between relaxation, transport and caged dynamics in a binary mixture on a per-component basis. J. Chem. Phys., 138:12A532, 2013.

[5] Emmanuel Guillaud, Laurent Joly, Dominique de Ligny, and Samy Merabia. Assessment of elastic models in supercooled water: A molecular dynamics study with the tip4p/2005f force field. The Journal of Chemical Physics, 147(1):014504, 2017.

[6] R. Horstmann and M. Vogel. Common behaviors associated with the glass transitions of water-like models. The Journal of Chemical Physics, 147(3):034505, 2017.

[7] Jack F. Douglas, Beatriz A. Pazmi˜no Betancourt, Xuhang Tong, and Hao Zhang. Localization model description of diffusion and structural relaxation in glass-forming cu–zr alloys. J. Stat. Mech.: Theory Exp., page 054048, 2016.

[8] F. Puosi, A. Pasturel, N. Jakse, and D. Leporini. Communication: Fast dynamics perspective on the breakdown of the stokes-einstein law in fragile glassformers. The Journal of Chemical Physics, 148(13):131102, 2018.

[9] A. Ottochian, C. De Michele, and D. Leporini. Universal divergenceless scaling between structural relaxation and caged dynamics in glass-forming systems. J. Chem. Phys., 131:224517, 2009.

[10] A. Ottochian and D. Leporini. Scaling between structural relaxation and caged dynamics

in ca0.4k0.6(no3)1.4 and glycerol: free volume, time scales and implications for the pressure-energy correlations. Phil. Mag., 91:1786–1795, 2011.

[11] F. Puosi and D. Leporini. Correlation of the instantaneous and the intermediate-time elasticity with the structural relaxation in glassforming systems. J. Chem. Phys., 136:041104, 2012.

[12] F. Puosi and D. Leporini. Communication: Fast and local predictors of the violation of the stokes- einstein law in polymers and supercooled liquids. J. Chem. Phys., 136:211101, 2012.

[13] Beatriz A. Pazmi˜no Betancourt, Paul Z. Hanakata, Francis W. Starr, and Jack F. Douglas. Quantitative relations between cooperative motion, emergent elasticity, and free volume in model glass-forming polymer materials. Proc. Natl. Acad. Sci. USA, 112:2966–2971, 2015.

[14] Matteo Becchi, Andrea Giuntoli, and Dino Leporini. Molecular layers in thin supported films exhibit the same scaling as the bulk between slow relaxation and vibrational dynamics. Soft Matter, 14:8814–8820, 2018.

[15] Karolina Adrjanowicz, Roksana Winkler, Andrzej Dzienia, Marian Paluch, and Simone Napolitano. Connecting 1d and 2d confined polymer dynamics to its bulk behavior via density scaling. ACS Macro Letters, 8(3):304–309, 2019.

[16] F Puosi, N Jakse, and A Pasturel. Dynamical, structural and chemical heterogeneities in a binary metallic glass-forming liquid. Journal of Physics: Condensed Matter, 30(14):145701, 2018.

[17] Elijah Flenner and Grzegorz Szamel. Fundamental differences between glassy dynamics in two and three dimensions. Nature Communications, 6(1):7392, dec 2015.

[18] Bernd Illing, Sebastian Fritschi, Herbert Kaiser, Christian L. Klix, Georg Maret, and Peter Keim. Mermin– Wagner fluctuations in 2D amorphous solids. Proceedings of the National Academy of Sciences, 114(8):1856–1861, feb 2017.

[19] Steve Plimpton. Fast Parallel Algorithms for Short-Range Molecular Dynamics. Journal of Computational Physics, 117(1):1–19, mar 1995.

[20] M.I. Mendelev, M.J. Kramer, R.T. Ott, D.J. Sordelet, D. Yagodin, and P. Popel. Development of suitable interatomic potentials for simulation of liquid and amorphous Cu–Zr alloys. Philos. Mag., 89(11):967– 987, 2009.

[21] Yuan-Chao Hu, Hajime Tanaka, and Wei-Hua Wang. Impact of spatial dimension on structural ordering in metallic glass. PHYSICAL REVIEW E, 96:22613, 2017.

[22] Hayato Shiba, Peter Keim, and Takeshi Kawasaki. Isolating long-wavelength fluctuation from structural relaxation in two-dimensional glass: cage-relative displacement. Journal of Physics: Condensed Matter, page aaa8b8, 2018.

[23] Skanda Vivek, Colm P Kelleher, Paul M Chaikin, and Eric R Weeks. Long-wavelength fluctuations and the glass transition in two dimensions and three dimensions. Proceedings of the National Academy of Sciences of the United States of America, 114(8):1850–1855, feb 2017.

[24] A. Rahman. Correlations in the motion of atoms in liquid argon. Phys. Rev., 136:A405–A411, Oct 1964. [25] Hayato Shiba, Yasunori Yamada, Takeshi Kawasaki, and Kang Kim. Unveiling Dimensionality

Dependence of Glassy Dynamics: 2D Infinite Fluctuation Eclipses Inherent Structural Relaxation. Physical Review Letters, 117(24):245701, dec 2016.

[26] Asaph Widmer-Cooper, Heidi Perry, Peter Harrowell, and David R. Reichman. Irreversible reorganization in a supercooled liquid originates from localized soft modes. Nature Physics, 4(9):711–715, sep 2008. [27] Hao Zhang, Cheng Zhong, Jack F. Douglas, Xiaodong Wang, Qingping Cao, Dongxian Zhang, and

Jian-Zhong Jiang. Role of string-like collective atomic motion on diffusion and structural relaxation in glass forming Cu-Zr alloys. The Journal of Chemical Physics, 142(16):164506, apr 2015.

[28] F. Puosi, O. Chulkin, S. Bernini, S. Capaccioli, and D. Leporini. Thermodynamic scaling of vibrational dynamics and relaxation. The Journal of Chemical Physics, 145(23):234904, 2016.

[29] R. W. Hall and P. G. Wolynes. The aperiodic crystal picture and free energy barriers in glasses. J. Chem. Phys., 86:2943–2948, 1987.

[30] C. M. Roland, S. Hensel-Bielowka, M. Paluch, and R. Casalini. Supercooled dynamics of glass-forming liquids and polymers under hydrostatic pressure. Rep. Prog. Phys., 68:1405, 2005.

[31] M. C. C. Ribeiro, T. Scopigno, and G. Ruocco. Computer simulation study of thermodynamic scaling of dynamics of 2ca(no[sub 3])[sub 2] [center-dot] 3kno[sub 3]. J. Chem. Phys., 135:164510, 2011. [32] S Bernini, F Puosi, and D Leporini. Thermodynamic scaling of relaxation: insights from anharmonic